# Pb.pwd Specification-1963 (Specification (Notes & Tables))

Post on 11-Aug-2015

47 views

Embed Size (px)

DESCRIPTION

Pb.pwd Specification-1963 (Specification (Notes & Tables))TRANSCRIPT

<p>835</p>
<p>NOTES Note No. 1 METHOD OF DESIGN OF CEMENT CONCRETE MIXES Usually when cement concrete mix is specified for a particular job, fixed proportions of cement, sand and coarse aggregate are mentioned, viz., a mix of 1:4:8 is specified for foundation concrete, 1:2:4 for reinforced concrete, beams and slabs, etc. This arbitrary mix method has certain drawbacks as the exact strength of the arbitrary mix method as certain such mixes are usually uneconomical. For large-scale works where facilities for quality control are available, it is suggested that concrete of a stipulated strength is specified and economical mix is worked out by some rational method. The object of designing the concrete mix is to determine the most economical and practical combination of available aggregates cement, water and in some cases admixture and/or pozzolana that will produce a mixture having the required degree of workability and will develop the required qualities of durability and strength on hardening. The object of this note is to explain in a simple manner the method to be adopted for designing the concrete mix. It is a well established fact that water cement ratio determines the strength of concrete. With given materials and ratio of mix, it is only the ratio of quantity of water to the quantity of cement which determines the strength of concrete, provided the mix is of a workable plasticity (i.e. the concrete thus made is capable of being fully compacted). The strength of concrete does not depend upon the type of grading of the coarse and fine aggregates provided the concrete produced is fully compacted and does not have any voids left in it. Thus the proportions of coarse and fine aggregate and their grading is not important from strength point of view. It is important only from the point of view of economy. A well graded mix will require less quantity of water cement paste to give proper compaction and specified workability. Average crushing strength The first step in designing of concrete mix is to fix the average crushing strength for laboratory conditions. As the working conditions in the field are not as perfect as the conditions in a laboratory, the mix should be designed for greater strength than the minimum strength specified. There is always variation in actual laboratory conditions from ones existing in the field. We have, therefore, to design the concrete for greater strength in the laboratory so as to cover normal lapses in the field conditions. The relation between minimum and average crushing strengths of works cubes for different working conditions in the field are given in Table No. 1. For</p>
<p>836</p>
<p>works satisfying the condition of fair control with weight batching, the percentage between minimum and average crushing strength will be 60. For a minimum crushing strength of 3,000 lbs. p.s.i., the average crushing strength will be 3000/0.6 = 5,000 lb. p.s.i. and the mix will be designed in the laboratory for an average crushing strength of 5,000 lbs. p.s.i. The Indian Standard Code of Practice for R.C.C. work in buildings specifies that the crushing strength for which mix should be designed in the laboratory should be 1 times the strength actually required. This practice is recommended to be adopted for general building construction in the State wherein sufficient quality control can be exercised. Fixing Water Cement Ratio The next step is to fix cement water ratio for the average crushing strength. This ratio can be fixed from Abrams formula which is given below:14000 S= -----------4x Where S = the average crushing strength. X = W/C ratio by volume. For S = 5000 lbs./by volume. X=0.51 by volume from the above formula. Water cement ratio can be fixed from this formula or it can be read directly from Table No. 2. While fixing the water cement ratio, 28 days strength should be taken into account. The water cement ratio has also a bearing on the consideration of degree of exposure to which the concrete is to be subjected. The water cement ratio from this consideration is tabulated in Table No. 3. The lower of the two values of water cement ratio as given in Table No. 2 and Table No. 3 may be adopted. However, the minimum quantity of cement to be used in controlled concrete for R. C. C. work shall not be less than 12 cwt. per 100 cft. (220 kg. per cu. meter) of concrete. Fixing slump for the concrete mix. Having fixed the c/w ratio, we have to workability of concrete for which mix is designed. The workability and consistency of fix the to be</p>
<p>837 concrete is measured by the standard slump test. The slump for various working conditions has been recommended in paragraph 7 of specification no. 10.4 cement concrete for ordinary structures. Suitable slump may be chosen according to working conditions. In case of controlled concrete, mechanical vibrators must be used so that concrete with comparatively lower slump can be used and economy can be achieved in the use of water-cement paste. Fixing nominal size of coarse aggregate The next step is to fix the nominal size of coarse aggregate for use in the concrete. The size of aggregate may be chosen according to the provision made in paragraph 9 of specification 3.29 for coarse aggregate. Proportion of Aggregates Having fixed the water cement ratio, slump and nominal size of coarse aggregate, we have to determine the economical proportion for coarse and fine aggregates for which any of the following three methods may be adopted:I. Fineness Modulus Method The fineness modulus of coarse aggregate and fine aggregate is determined separately by sieving them through the following set of sieves and recording result as below:Size of sieve 1 3 1 3/8 3/16 No. 7 No. 14 No. 25 No. 50 No. 100 Total Weight of Weight of aggregate aggregate retained coarser than 2 3 Percentage of material coarser than 4</p>
<p>838 The total of column 4 divided by 100 will give F. M. Let F. M. of coarse aggregate be called A and F. M. of fine aggregate be called C and let the economical value of F. M. for combined aggregate be called B. The economical value of combined aggregate can be obtained from Table No. 4. The percentage of fine aggregate to combined aggregate can be worked out from the formula given below:P = 100X___A-B___ A-C This will fix the proportions of fine aggregate to coarse aggregate. Determining the quantity of cement paste required Having fixed the water cement ratio and the proportion of fine aggregate to coarse aggregate, we have now to determine the quantity of water cement paste to be added to the combined aggregate to get the required workability which can be tested by the slump test. An easy and practical method is to prepare a number of batches of combined aggregate in the proportion fixed and add varying quantities of water-cement paste having the fixed water cement ratio to get the required slump. To start with, the least quantity of water is added to the first batch. This least quantity of water can be determined from the following formula:0.3 X plus 0.1 Y plus 0.01 Z=W/C XX Where X = quantity of cement by weight. Y = quantity of fine aggregate by weight. Z = quantity of coarse aggregate by weight. And W/C = Water Cement ratio. To take a practical example, let us suppose F.M. of coarse aggregate to be 6.42 and F.M. of fine aggregate to be 1.78. The average F.M. of combined aggregate for size is 4.90 according to Table No. 4. Then P = 32.7 per cent; that means fine aggregate should be 32.7% of the combined aggregate by weight and coarse aggregate should be 67.3%. Taking 50 lbs. of coarse aggregate, the weight of fine aggregate 50 x 32.7 required is --------------- = Four or five samples of combined 67.3</p>
<p>839 aggregate in the above proportion may be prepared by weighing. Let the water cement ratio be 0.51 then the minimum quantity of water for harsh mix is worked out as under :0.3 x plus 0.1 x 24.3 plus 0.01 x 50 = 0.51 x X = 14 lbs Water required 14 X 0.51 = 7 lbs. (app). Mix 14 lbs of cement and 7 lbs. of water with the first batch of combined aggregate and carry out slump test. The slump may be zero. Then add 15 lbs. of cement and 7 lbs. of water with the second batch of combined aggregate and test the slump which may be . Go on increasing the quantity of cement by half a lb. and quantity of water by lb. till the required slump has obtained. Let us suppose the required slump was obtained with 15 lbs. of cement and 7 lbs. of water. From this ratio of cement, fine aggregate coarse aggregate works out by weight to 15.5 : 24.3 : 50 which is equal to 1:1. 58:3.23. This proportion can be used in case weight batching is done. In case mixing is to be done by volume, then the above proportion can be easily converted into proportion by volume. II. Optimum percentage of sand method In this method, the water-cement ratio, the size of aggregate and slump are fixed as detailed above. Coarse and Fine aggregates are mixed in various arbitrary proportions and quantity of water cement paste required is worked out in each case to give the required slump. This is done as described in the above method. When the required slump has been obtained the quantity of concrete thus made is filled into steel cubes and the quantity of cement, concrete produced is measured. As an example, fine and coarse aggregates may be fixed in the proportions 25 to 75, 30 to 70 and 35 to 65.The results are recorded as follows:Percent Weig Weig age of ht of ht of F.A. C.A. sand and C.A. Weight of cement added to get 1 slump lbs. 11.0 11.5 12.5 Weig ht of water adde d Volum e of ceme nt obtain ed lbs. 0.485 0.520 0.542 Weight of cement per cft. Of concret e Cft. 22.7 23.0 23.0 %age of sand/C. A.</p>
<p>lbs. 25.75 30.70 35.65 45 42 39</p>
<p>lbs. 15 18 21</p>
<p>lbs. 5.5 5.75 6.25</p>
<p>lbs. 33% 43% 54%</p>
<p>840 For all these three samples, the weight of cement per cft. of concrete is worked out as well as the percentage of sand over the quantity of coarse aggregate. A graph is plotted with percentage of sand over the coarse aggregate as abscissa and lbs. of cement per cft. of concrete as ordinate. The lowest portion of this curve gives an optimum percentage of sand as shown in figure given below:-</p>
<p>It shows that when the percentage of sand to coarse aggregate is 43, minimum quantity of cement is required to produce 1 cft. of concrete. This shows that this percentage of sand gives the minimum amount of voids and surface area in the concrete and gives the most economical mix. According to figures mentioned above, the proportion of cement : fine aggregate : coarse aggregate work out to 11 : 5 : 18 : 42 by weight which may be converted into proportion by volume if weigh batching is not to be done in the field. III Arbitrary Method for Concrete Mix Design In this method, the average crushing strength required for laboratory conditions, the net water cement ratio required for concrete and the slump required for various types of sections and the maximum size of aggregate to be used are determined as previously described. The approximate sand and water contents per cu. yd, concrete are found out from Table No 5. Necessary adjustments for the values of sand content and</p>
<p>841</p>
<p>water content are made for the variables such as water cement ratio, F.M. of sand, and for slump, etc. The procedure is illustrated by means of an example. As an example, consider that a project involves an ordinary heavily reinforced retaining wall having a minimum thickness of 6. The wall has been designed on the basis of a cube crushing strength of 4,000 lbs. per sq. in at 28 days. It is proposed that the concrete will be controlled very accurately with weigh batching and good supervision will be carried out. The fine aggregate available at site has F.M. of 2.65 and the specific gravity of coarse aggregate is 2.8 (saturated surface dry) and the specific gravity of sand is 2.65 (saturated surface dry). The specific gravity of cement is 3.15 (assumed). Proportions of trail mix using rounded coarse, aggregate required are:(1) Average crushing strength 4000 x 100 = ------------------75 = 5350, say 5400 psi = 1 inch = 2 inch (3) Water cement ratio from Table 2 for strength of 5,400 psi. (4) From Table NO. 5, for a maximum size coarse aggregate Sand percentage of total aggregate by absolute volume = 0.49 = 1 inch = 41%</p>
<p>(2) Maximum size of aggregate</p>
<p>Net water content per cu. yd. in lbs. = 300. Adjustment due to variation in slump, water cement ratio and F.M. of sand etc.:Change in condition (a) For 0.08% decrease in W/C (percent sand) - 1.6 Unit water content 0 0 - 3% - 3% = 38.9% = 291 lbs.</p>
<p>(b) For 0.1 decrease in F.M. of - 0.5 sand (c) For 1 decrease of slump Total correction Sand content Water content 0 - 2.1% = 41 21 = 300 3x300 100</p>
<p>5. Final proportions of sand and water content:-</p>
<p>842 Net water content = -----------------------------Water cement ratio 291 = ---------- - 594 lbs per cu. yd. 0.49 594 = ---------- = 5.30 bags per cu. yd. 112 water content cement content = -------------------plus--------------------62.4 specific x 62.4 gravity 291 594 = ------- plus --------------------62.4 3.15 x 62.4 = 4.66 plus 3.04 = 7.70 cft. per cu. yd of concrete = 27 7.7 = 19.3 cft. per cu. yd. of concrete Absolute volume = percent sand x total aggregate = 0.398 7.7 = 19.3 cft. cu. yd. of concrete = Absolute volume - Absolute Total aggregate Volume sand = 19.3 19.3 = 11.8 cft. per cu. yd. of concrete = Absolute Volume x specific gravity x 62.4 = 7.5 x 2.65 x 62.4 = 1240 lb. cu. yd. of concrete = 11.8 x 2.8 x 62.4 = 20.60 lbs. per cu. yd. of concrete</p>
<p>6. Cement content</p>
<p>7.</p>
<p>(Absolute Volume, (Water plus cement)</p>
<p>8. 9.</p>
<p>Absolute Volume total aggregate Absolute Volume, sand Absolute Volume, Coarse aggregate Sand Cement</p>
<p>10.</p>
<p>11. 12.</p>
<p>Coarse aggregate content 13. Trial mix proportions: by weight 594 1240 2060 = ------- : ------------- - ---------- = 1 : 209 : 3.49 594 594 594 Say 1 : 2.1 : 3.5</p>
<p>843</p>
<p>TABLE 1 Estimated relation between the minimum and average crushing strength of work cubes for different work conditions Minimum strength of percentage of average strength 75 60 40</p>
<p>Work conditions</p>
<p>Very good control with weight batching, moisture determination of aggregates, etc. constant supervision Fair control with weight batching Poor control on volume of aggregate</p>
<p>844</p>
<p>TABLE 2 Compressive strengths for various water-cement ratio (Ordinary and Rapid Hardening Cements) Net water-Cement Ratio Gallons per bag of cement 4 4 5 5 6 6 7 7 8 8 Probable Crushing strength, PSI Ordinary Portland 7 days 5,600 5,000 4,300 3,700 3,200 2,800 2,400 2,100 1,800 1,600 28 days 7,300 6,700 6,000 5,400 4,700 4,200 3,700 3,300 3,000 2,700 Rapid hardening Portland 7 days 6,800 6,000 5,400 4,800 4,100 3,700 3,200 2,900 2,600 2,400 28 days 8,400 7,700 6,900 6,300 5,600 5,100 4,500 4,100 3,600 3,300</p>
<p>By weight</p>
<p>0.36 0.40 0.45 0.49 0.54 0.58 0.63 0.67 0.72 0.76</p>
<p>845</p>
<p>TABLE 3 Net water-cement ratios for various types of construction and exposure conditions...</p>

Recommended

Accountant's Handbook of Formulas and Tables-1963-Lawrence Lipkin, Irwin k.feinstein, Lucile Derrick